#------------------------------------------------------------------------------
#$Date: 2019-12-25 22:05:48 +0200 (Wed, 25 Dec 2019) $
#$Revision: 245834 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/31/13/2311373.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2311373
loop_
_publ_author_name
'Schwendtner, Karolina'
'Kolitsch, Uwe'
_publ_section_title
;
 New M⁺, M³⁺-arsenates - the framework
 structures of AgM³⁺(HAsO₄)₂
 (M³⁺ = Al, Ga) and
 M⁺GaAs₂O₇ (M⁺ =
 Na, Ag).
;
_journal_issue                   'Pt 5'
_journal_name_full
'Acta crystallographica. Section E, Crystallographic communications'
_journal_page_first              785
_journal_page_last               790
_journal_paper_doi               10.1107/S2056989017005631
_journal_volume                  73
_journal_year                    2017
_chemical_formula_iupac          'Ag Ga (H As O4)2'
_chemical_formula_structural     'Ag1 Ga1 (H1 As1 O4)2'
_chemical_formula_sum            'Ag As2 Ga H2 O8'
_chemical_formula_weight         457.45
_chemical_name_common            'silver gallium hydrogen arsenate'
_chemical_name_systematic        'Silver(I) gallium bis[hydrogen arsenate(V)]'
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2016/6
_cell_angle_alpha                90
_cell_angle_beta                 107.77(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.826(2)
_cell_length_b                   10.216(2)
_cell_length_c                   8.694(2)
_cell_measurement_reflns_used    1519
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      34.972
_cell_measurement_theta_min      2.037
_cell_volume                     661.9(3)
_computing_cell_refinement
;
HKL SCALEPACK (Otwinowski et al.,  2003)
;
_computing_data_collection
;
COLLECT (Nonius, 2003)
;
_computing_data_reduction
;
HKL DENZO and SCALEPACK (Otwinowski et al.,  2003)
;
_computing_molecular_graphics
;
DIAMOND (Brandenburg, 2005)
;
_computing_publication_material
;
publCIF (Westrip, 2010)
;
_computing_structure_refinement
;
SHELXL2016 (Sheldrick, 2015)
;
_computing_structure_solution
;
SHELXS97 (Sheldrick, 2008)
;
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Nonius KappaCCD single-crystal four-circle'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0120
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            2852
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         34.969
_diffrn_reflns_theta_min         3.384
_exptl_absorpt_coefficient_mu    16.957
_exptl_absorpt_correction_T_max  0.2819
_exptl_absorpt_correction_T_min  0.1503
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
(HKL SCALEPACK; Otwinowski et al.,  2003)
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    4.590
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'large pseudo-dipyramidal glassy'
_exptl_crystal_F_000             840
_exptl_crystal_size_max          0.180
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.100
_refine_diff_density_max         0.658
_refine_diff_density_min         -0.503
_refine_ls_extinction_coef       0.0133(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method
;
SHELXL2016 (Sheldrick, 2015)
;
_refine_ls_goodness_of_fit_ref   1.146
_refine_ls_hydrogen_treatment    refall
_refine_ls_matrix_type           full
_refine_ls_number_parameters     73
_refine_ls_number_reflns         1460
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.146
_refine_ls_R_factor_all          0.0160
_refine_ls_R_factor_gt           0.0147
_refine_ls_shift/su_max          0.037
_refine_ls_shift/su_mean         0.003
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0150P)²+0.9400P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0362
_refine_ls_wR_factor_ref         0.0366
_reflns_number_gt                1402
_reflns_number_total             1460
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            pk2600sup1.cif
_cod_data_source_block           AgGaHAsO42
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               2311373
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.150
_shelx_estimated_absorpt_t_max   0.282
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_occupancy
Ag Ag1 0.250000 0.250000 0.000000 0.0335(9) Uani d 0.75(2)
Ag Ag2 0.284(3) 0.2351(14) 0.019(2) 0.0316(18) Uani d 0.123(10)
Ga Ga 0.000000 0.13670(2) 0.250000 0.00500(5) Uani d 1
As As 0.27567(2) 0.39556(2) 0.35733(2) 0.00482(5) Uani d 1
O O1 0.18942(15) 0.26190(10) 0.24943(13) 0.00983(18) Uani d 1
O O2 0.32045(15) 0.49738(11) 0.22405(13) 0.01055(19) Uani d 1
O O3 0.45491(14) 0.35629(11) 0.51333(13) 0.00948(18) Uani d 1
O O4 0.11608(16) 0.46896(14) 0.42534(15) 0.0169(2) Uani d 1
H H 0.148(4) 0.487(3) 0.519(4) 0.033(8) Uiso d 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O1 Ga O1 . 2 98.48(7)
O1 Ga O2 . 3_445 171.19(5)
O1 Ga O2 2 3_445 87.59(5)
O1 Ga O2 . 4_545 87.59(5)
O1 Ga O2 2 4_545 171.19(5)
O2 Ga O2 3_445 4_545 87.12(7)
O1 Ga O3 . 7_556 94.82(5)
O1 Ga O3 2 7_556 82.46(5)
O2 Ga O3 3_445 7_556 92.29(5)
O2 Ga O3 4_545 7_556 90.71(5)
O1 Ga O3 . 8_455 82.46(5)
O1 Ga O3 2 8_455 94.82(5)
O2 Ga O3 3_445 8_455 90.71(5)
O2 Ga O3 4_545 8_455 92.29(5)
O3 Ga O3 7_556 8_455 175.86(6)
O2 As O3 . . 114.16(6)
O2 As O1 . . 104.63(6)
O3 As O1 . . 110.64(6)
O2 As O4 . . 107.25(7)
O3 As O4 . . 110.16(6)
O1 As O4 . . 109.80(6)
O2 As O3 . . 114.16(6)
O2 As O1 . . 104.63(6)
O3 As O1 . . 110.64(6)
O2 As O4 . . 107.25(7)
O3 As O4 . . 110.16(6)
O1 As O4 . . 109.80(6)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Ag1 O1 7 2.3600(12) n
Ag1 O1 . 2.3600(12) y
Ag1 O3 2_655 2.5864(12) y
Ag1 O3 8_455 2.5864(12) n
Ag1 O4 6_565 3.0574(15) y
Ag1 O4 4_545 3.0574(15) n
Ag1 O2 . 3.1352(12) y
Ag2 O1 . 2.357(17) y
Ag2 O1 7 2.402(18) y
Ag2 O3 2_655 2.48(2) y
Ag2 O3 8_455 2.73(3) y
Ag2 O4 4_545 2.83(2) y
Ag2 O2 7 3.116(18) y
Ag2 O2 . 3.185(17) y
Ga O1 . 1.9591(11) y
Ga O1 2 1.9591(11) n
Ga O2 3_445 1.9641(11) y
Ga O2 4_545 1.9641(11) n
Ga O3 7_556 1.9799(12) y
Ga O3 8_455 1.9799(12) n
As O2 . 1.6719(11) y
As O3 . 1.6753(12) y
As O1 . 1.6773(11) y
As O4 . 1.7096(12) y
O4 H . 0.80(3) ?
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
O4 H O2 6_566 0.80(3) 1.89(3) 2.6240(19) 153(3)
